Thermo-mechanical coupling and size effects in micro and nano resonators
© Kumar et al.; licensee Springer. 2013
Received: 18 March 2013
Accepted: 29 June 2013
Published: 6 August 2013
Existing models for thermoelastic damping consider geometric size effects only, the focus of this study is on tuning of thermoelastic damping with mechanical strain, which reduces both relaxation rate and thermal conductivity at the nanoscale. We developed a model that accounts for the contribution of tensile force and thermal conductivity in a clamped-clamped configuration nano-resonator. Experimentally measured thermal conductivity is then coupled with the model suggests the existence of a critical length scale (inversion point) below which quality factor increases with increase in thickness and vice versa. The nanoscale strain-thermal conductivity coupling is found to be most effective at and around this inversion point.
The ever continuing pursuit for high-precision and low power consumption micro and nano electro-mechanical systems (MEMS and NEMS) actuators, sensors and mechanical filter applications has resulted in increasing attention on resonators used in these devices . Quality factor (Q-factor) is one of the critical performance parameters for resonators, which is influenced by various kinds of energy loss mechanisms and majority of the micro/nano resonator research is devoted on the size and design effects to understand or suppress such mechanisms. Decreasing geometrical dimensions has conducive effects on sensitivity and dynamics of resonators; however energy loss has been observed to increase with decreasing size . Air damping, thermoelastic damping and other losses at the supports and surfaces [3–5] are the primary energy loss mechanisms. Thermoelastic damping, resulting from heat generation due to vibration and dissipation from thermal diffusion, is identified as the fundamental limit for the attainable quality factor of a micromechanical resonator . This is because the literature has only insights on the basic processes of thermo-elastic damping, but there is no effective theory that is capable of reducing the loss around the Debye peak (where resonator frequency is on the order of the relaxation rate) .
Very recently, the concept of mechanical pre-stress (or strain) as a mechanism for decreasing thermo-elastic damping was introduced and discussed . Here, the active tension in the resonator beam is found to increase the frequency but also more importantly decrease the relaxation rate, thereby decreasing the overall thermo-elastic damping in the system. The mechanical strain can be applied during fabrication (for example, the tensile residual stress of silicon nitride can be exploited ) as well as with external control during device operation. Previously, we developed a model that explicitly relates the Q-factor with the tensile force . The core theme of the present study however is a novel concept that further reduction in thermoelastic damping is possible by controlling the heat dissipation. This concept is yet to appear in the literature, where it is well established that thermal conductivity (and hence heat dissipation) is invariant with applied strain [11, 12]. We argue that this is true only at larger length-scales but at nanoscale, mechanical and thermal properties may be strongly coupled [13, 14]. Motivated by the recent observations of unprecedented size induced mechanical strain-thermal conductivity coupling [15, 16], we propose that for nanoscale resonators, it may be possible to tune the thermo-elastic dissipation with applied strain. In this paper, we investigate this hypothesis by experimentally measuring the variation in thermal conductivity as a function of uniaxial stress and then applying the data on a theoretical model relating thermo-elastic damping to mechanical pre-stress and thermal conductivity.
When inserted to Equation (2), the above expression shows that thermoelastic damping is dependent upon thermal conductivity as well as specific heat. Both of these are commonly known to be intrinsic properties of materials, hence there are no attempts in the literature to exploit the variation of these properties to reduce the thermo elastic damping. This is questionable at the nanoscale, where thermal and mechanical properties are very different from the bulk. Therefore, we shift the focus to the nanoscale, where these properties are not only different, but also very strongly coupled. Our previous studies indicate that thermal conductivity is dependent on the applied mechanical strain, which we propose to exploit as a thermoelastic damping tuning parameter. In the next section, we describe an experimental study to validate this critical assumption by characterizing the relationship between strain and thermal conductivity for silicon nitride. This material has been studied in nanoscale resonators with various levels of applied mechanical pre-strain and thus is most relevant to this paper.
Our goal in current work is to understand the coupling between mechanical strain and thermal conductivity. This coupling data will then be utilized to theoretically understand the thermoelastic damping in micro resonators. In order to address this goal, we need to develop an experimental setup that can apply mechanical strain while thermal conductivity measurements are being done. We utilized the thin film residual stress (self actuation) to apply mechanical loading on the specimen. We carried out experiments on Si3N4 beams to find out strain dependence of thermal conductivity. But brittle behavior and large residual stresses make characterization of Si3N4 extremely challenging.
Thermal conductivity of the freestanding thin film specimen is measured by a direct steady state technique that involves the temperature gradient along the length of the specimen and the heat flux while the specimen when it is heated by a microheater. The thin film metal heater line is also freestanding and is perpendicular to the specimen as shown in Figure 1. Thermal conductivity measurement process starts with the passage of direct current, typically 4-10 mA, through the aluminum metal line. It produces a parabolic temperature profile in the freestanding part of the heater line due to the Joule heating and develops the maximum temperature region in the intersection of aluminum heater and silicon nitride specimen. The temperature profiles along the length of heater and specimen are mapped by using an infrared microscope (Quantum Focus Instruments, MWIR-512 InSb IR FPA camera) with 0.1 K temperature and 2 μm spatial resolution. The measured temperature profile of the specimen is used to calibrate a finite element model of the device. After such calibration, the heat flux from the aluminum heater to the nitride specimen and the thermal conductivity of the specimen can be calculated by finite element analysis. We used COMSOL Multiphysics™ to carry out the finite element simulations. First, heater line is modeled by using known input parameters, such as heat transfer coefficient through that air; electrical resistivity, temperature coefficient of resistance and thermal conductivity of heater material. The temperature profile of heater thus obtained from the simulation is found in very good agreement with the measured temperature profile by IR microscope. Then heat flux values from heater to specimen for different input currents are obtained from the simulation results. These heat flux values are then used with the temperature gradient in the specimen to obtain thermal conductivity using the Fourier’s law. Further details of the procedure is given in reference .
Results and discussion
One critical observation that can be derived from Equation 2 is dependence of thermoelastic damping on ratio of thickness to length. Increase in length while keeping the thickness changes this ratio and results in decrease in Q-factor or increase in thermoelastic damping.
A survey of these different plots suggests that applied strain is very effective way of modifying natural frequency as well as Q-factor of the resonator with geometry very close to inversion point for any particular length. But the strain effect is not really pronounced when we are either far right or left of this point. While the present study delineates the influence of thermal conductivity tuning with mechanical strain in resonators, direct experimental validation is extremely difficult. This is because it is not possible to measure thermo-elastic damping exactly. A more tractable quantity is the Q factor, but it depends on various types of dissipation mechanisms (surface, clamping boundary conditions) and it is impossible to experimentally isolate these losses to quantify the thermoelastic damping contribution. We therefore are unable to present the direct measurement of the thermo-elastic damping with the tuned thermal conductivity in this study.
From Zener’s work we know that the thermoelastic damping is a function of natural frequency and thermal relaxation time constant. It is also known that natural frequency vary with size as well as applied mechanical strain and thermal relaxation time constant is a function of thermal properties. But current theoretical models for thermoelastic damping consider only geometric size effects and neglect the corresponding size effects that exist for mechanical and thermal properties. We utilized a combined experimental and theoretical approach to explore thermoelastic damping size effects arising from coupling of mechanical strain and thermal conductivity. In this work, the affect of mechanical strain on SiN thin films is experimentally explored. It is found that thermal conductivity degrades significantly with increase in mechanical strain. Further, it is observed that mechanical pre-strain can strongly improve quality factor by not only increasing the natural frequency and decreasing the relaxation rate, but also by decreasing the thermal conductivity. We also found that consideration of strain and thermal conductivity lead to the existence of a critical length scale (inversion point) below which quality factor increases with increase in thickness and vice versa. The nanoscale strain-thermal conductivity coupling is found to be most effective at and around this inversion point.
M.A. Haque gratefully acknowledges the support from the Center for Nanoscale Mechatronics & Manufacturing of the Korea Institute of Machinery & Materials and the National Science Foundation, USA (CMMI # 1029935).
- Yi YB: Geometric effects on thermoelastic damping in MEMS resonators. J Sound Vib 2008,309(3–5):588–599.View ArticleGoogle Scholar
- Duwel A, et al.: Engineering MEMS resonators with low thermoelastic damping. Journal of Microelectromechanical Systems 2006,15(6):1437–1445.View ArticleGoogle Scholar
- Mihailovich RE, MacDonald NC: Dissipation measurements of vacuum-operated single-crystal silicon microresonators. Sensors and Actuators A 1995, 50: 199–207. 10.1016/0924-4247(95)01080-7View ArticleGoogle Scholar
- Zhang C, Xu G, Jiang Q: Analysis of the air-damping effect on a micromachined beam resonator. Mathematics and Mechanics of Solids 2003,8(3):315–325. 10.1177/1081286503008003006View ArticleGoogle Scholar
- Hao Z, Ayazi F: Support loss in the radial bulk-mode vibrations of center-supported micromechanical disk resonators. Sensors and Actuators, A 2007,134(2):582–593. 10.1016/j.sna.2006.05.020View ArticleGoogle Scholar
- Lifshitz R, Roukes ML: Thermoelastic damping in micro- and nanomechanical systems. Physical Review B 2000,61(8):5600. 10.1103/PhysRevB.61.5600View ArticleGoogle Scholar
- Zener C, 3: Internal friction in solids. I. Theory of internal friction in reeds. Phys Rev 1937, 52: 230. 10.1103/PhysRev.52.230View ArticleGoogle Scholar
- Kumar S, Aman Haque M, 1: Stress-dependent thermal relaxation effects in micro-mechanical resonators. Acta Mechanica 2010, 212: 83–91. 10.1007/s00707-009-0244-6View ArticleGoogle Scholar
- Irene E: Residual stress in silicon nitride films. J Electron Mater 1976,5(3):287–298. 10.1007/BF02663273View ArticleGoogle Scholar
- Kumar S, Haque MA: Reduction of thermo-elastic damping with a secondary elastic field. J Sound Vib 2008,318(3):423–427. 10.1016/j.jsv.2008.06.039View ArticleGoogle Scholar
- Tritt TM (Ed): Thermal conductivity: theory, properties, and applications. Springer, US; 2004.Google Scholar
- Anderson CVDR, Tamma KK: An overview of advances in heat conduction models and approaches for prediction of thermal conductivity in thin dielectric films. International Journal of Numerical Methods for Heat & Fluid Flow 2004,14(1):12–65. 10.1108/09615530410511621View ArticleGoogle Scholar
- Feng B, Li Z, Zhang X: Prediction of size effect on thermal conductivity of nanoscale metallic films. Thin Solid Films 2009,517(8):2803–2807. 10.1016/j.tsf.2008.10.116MathSciNetView ArticleGoogle Scholar
- Arzt E: Size effects in materials due to microstructural and dimensional constraints: a comparative review. Acta Mater 1998,46(16):5611–5626. 10.1016/S1359-6454(98)00231-6View ArticleGoogle Scholar
- Lee HF, Kumar S, Haque MA: Role of mechanical strain on thermal conductivity of nanoscale aluminum films. Acta Mater 2010,58(20):6619–6627. 10.1016/j.actamat.2010.08.024View ArticleGoogle Scholar
- Alam MT, et al.: Influence of strain on thermal conductivity of silicon nitride thin films. J Micromech Microeng 2012,22(4):045001. 10.1088/0960-1317/22/4/045001MathSciNetView ArticleGoogle Scholar
- Zener C: Internal friction in solids II. General theory of thermoelastic internal friction. Phys Rev 1938,53(1):90. 10.1103/PhysRev.53.90View ArticleGoogle Scholar
- Zener C, Otis W, Nuckolls R: Internal friction in solids III. Experimental demonstration of thermoelastic internal friction. Phys Rev 1938,53(1):100. 10.1103/PhysRev.53.100View ArticleGoogle Scholar
- Zener C: Internal friction in solids. Proceedings of the Physical Society 1940,52(1):152–166. 10.1088/0959-5309/52/1/322View ArticleGoogle Scholar
- Nayfeh AH, Younis MI: Modeling and simulations of thermoelastic damping in microplates. J Micromech Microeng 2004,14(12):1711–1717. 10.1088/0960-1317/14/12/016View ArticleGoogle Scholar
- Rajagopalan J, Saif MTA: Single degree of freedom model for thermoelastic damping. Journal of Applied Mechanics, Transactions ASME 2007,74(3):461–468. 10.1115/1.2338054View ArticleGoogle Scholar
- Guo FL, Rogerson GA: Thermoelastic coupling effect on a micro-machined beam resonator. Mech Res Commun 2003,30(6):513–518. 10.1016/S0093-6413(03)00061-2View ArticleGoogle Scholar
- Landau LD, Lifshitz EM: Theory of elasticity. 3rd ed. Course of Theoretical Physics 2007, 7: 133–143. Butterworth Heinemann,Google Scholar
- Bokaian A: Natural frequencies of beams under tensile axial loads. J Sound Vib 1990,142(3):481–498. 10.1016/0022-460X(90)90663-KView ArticleGoogle Scholar
- Poetzsch RHH, Bottger H, 21: Interplay of disorder and anharmonicity in heat conduction: molecular-dynamics study. Physical Review B 1994, 50: 15757–15763. 10.1103/PhysRevB.50.15757View ArticleGoogle Scholar
- Allen PB, Feldman JL: Thermal conductivity of disordered harmonic solids. Physical Review B 1993,48(17):12581–12588. 10.1103/PhysRevB.48.12581View ArticleGoogle Scholar
- Alexander S, Entin-Wohlman O, Orbach R: Phonon-fracton anharmonic interactions: The thermal conductivity of amorphous materials. Physical Review B 1986,34(4):2726. 10.1103/PhysRevB.34.2726View ArticleGoogle Scholar
- Allen PB, et al.: Diffusons, locons and propagons: character of atomic vibrations in amorphous Si. Philosophical Magazine Part B 1999,79(11–12):1715–1731.View ArticleGoogle Scholar
- Verbridge SS, et al.: Macroscopic tuning of nanomechanics: substrate bending for reversible control of frequency and quality factor of nanostring resonators. Nano Lett 2007,7(6):1728–1735. 10.1021/nl070716tView ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.